Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this presentation? Why not share!

No Downloads

Total views

5,652

On SlideShare

0

From Embeds

0

Number of Embeds

8

Shares

0

Downloads

578

Comments

0

Likes

11

No embeds

No notes for slide

- 1. FUNDAMENTALS OF METAL CASTING <ul><li>Overview of Casting Technology </li></ul><ul><li>Heating and Pouring </li></ul><ul><li>Solidification and Cooling </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 2. Solidification Processes <ul><li>Starting work material is either a liquid or is in a highly plastic condition, and a part is created through solidification of the material </li></ul><ul><li>Solidification processes can be classified according to engineering material processed: </li></ul><ul><ul><li>Metals </li></ul></ul><ul><ul><li>Ceramics, specifically glasses </li></ul></ul><ul><ul><li>Polymers and polymer matrix composites (PMCs) </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 3. <ul><li>Classification of solidification processes </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 4. Casting of Metals <ul><li>Process in which molten metal flows by gravity or other force into a mold where it solidifies in the shape of the mold cavity </li></ul><ul><li>The term casting also applies to the part made in the process </li></ul><ul><li>Steps in casting seem simple: </li></ul><ul><ul><li>Melt the metal </li></ul></ul><ul><ul><li>Pour it into a mold </li></ul></ul><ul><ul><li>Let it freeze </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 5. Equation 10.1 H = ρ V{C s (T m – T o ) + H f + C l (T p –T m )} <ul><li>H = Total heat required </li></ul><ul><li>ρ = density, g/cm 3 or lbs/in 3 </li></ul><ul><li>V = volume of metal being heated, cm 3 or in 3 </li></ul><ul><li>C s = weight specific heat of solid metal J/g-C or Btu/lb-F </li></ul><ul><li>T m = melting temperature, C or F </li></ul><ul><li>T o = starting temperature, C or F </li></ul><ul><li>T p = pouring temperature, C or F </li></ul><ul><li>H f = heat of fusion J/g or Btu/lb </li></ul><ul><li>C l = weight specific heat of liquid metal J/g-C or Btu/lb-F </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 6. <ul><li>A sufficient amount of pure copper is to be heated for casting a large plate in an open mold. The plate has dimensions: length = 20 in, width = 10 in, and thickness = 3 in. Compute the amount of heat that must be added to the metal to heat it to a temperature of 2150°F for pouring. Assume that the amount of metal heated will be 10% more than what is needed to fill the mold cavity. Properties of the metal are: density = 0.324 lbm/in 3 , melting point = 1981°F, specific heat of the metal = 0.093 Btu/lbm-F in the solid state and 0.090 Btu/lbm-F in the liquid state; and heat of fusion = 80 Btu/lbm. </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 7. Capabilities and Advantages of Casting <ul><li>Can create complex part geometries </li></ul><ul><li>Can create both external and internal shapes </li></ul><ul><li>Some casting processes are net shape; others are near net shape </li></ul><ul><li>Can produce very large parts </li></ul><ul><li>Some casting methods are suited to mass production </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 8. Disadvantages of Casting <ul><li>Different disadvantages for different casting processes: </li></ul><ul><ul><li>Limitations on mechanical properties </li></ul></ul><ul><ul><li>Poor dimensional accuracy and surface finish for some processes; e.g., sand casting </li></ul></ul><ul><ul><li>Safety hazards to workers due to hot molten metals </li></ul></ul><ul><ul><li>Environmental problems </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 9. Parts Made by Casting <ul><li>Big parts </li></ul><ul><ul><li>Engine blocks and heads for automotive vehicles, wood burning stoves, machine frames, railway wheels, pipes, church bells, big statues, pump housings </li></ul></ul><ul><li>Small parts </li></ul><ul><ul><li>Dental crowns, jewelry, small statues, frying pans </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 10. Overview of Casting Technology <ul><li>Casting is usually performed in a foundry </li></ul><ul><li>Foundry = factory equipped for making molds, melting and handling molten metal, performing the casting process, and cleaning the finished casting </li></ul><ul><li>Workers who perform casting are called foundrymen </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 11. The Mold in Casting <ul><li>Contains cavity whose geometry determines part shape </li></ul><ul><ul><li>Actual size and shape of cavity must be slightly enlarged to allow for shrinkage of metal during solidification and cooling </li></ul></ul><ul><ul><li>Molds are made of a variety of materials, including sand, plaster, ceramic, and metal </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 12. Open Molds and Closed Molds <ul><li>Two forms of mold: (a) open mold and (b) closed mold for more complex mold geometry with gating system leading into the cavity </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 13. Two Categories of Casting Processes <ul><li>Expendable mold processes – use an expendable mold which must be destroyed to remove casting </li></ul><ul><ul><li>Mold materials: sand, plaster, and similar materials, plus binders </li></ul></ul><ul><li>Permanent mold processes – use a permanent mold which can be used to produce many castings </li></ul><ul><ul><li>Made of metal (or, less commonly, a ceramic refractory material </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 14. Advantages and Disadvantages <ul><li>More intricate geometries are possible with expendable mold processes </li></ul><ul><li>Part shapes in permanent mold processes are limited by the need to open the mold </li></ul><ul><li>Permanent mold processes are more economic in high production operations </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 15. Sand Casting Mold ©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 16. Terminology for Sand Casting Mold <ul><li>Mold consists of two halves: </li></ul><ul><ul><li>Cope = upper half of mold </li></ul></ul><ul><ul><li>Drag = bottom half </li></ul></ul><ul><li>Mold halves are contained in a box, called a flask </li></ul><ul><li>The two halves separate at the parting line </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 17. Forming the Mold Cavity in Sand Casting <ul><li>Mold cavity is formed by packing sand around a pattern , which has the shape of the part </li></ul><ul><li>When the pattern is removed, the remaining cavity of the packed sand has desired shape of cast part </li></ul><ul><li>The pattern is usually oversized to allow for shrinkage of metal during solidification and cooling </li></ul><ul><li>Sand for the mold is moist and contains a binder to maintain its shape </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 18. Use of a Core in the Mold Cavity <ul><li>The mold cavity provides the external surfaces of the cast part </li></ul><ul><li>In addition, a casting may have internal surfaces, determined by a core , placed inside the mold cavity to define the interior geometry of part </li></ul><ul><li>In sand casting, cores are generally made of sand </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 19. Gating System <ul><li>Channel through which molten metal flows into cavity from outside of mold </li></ul><ul><li>Consists of a downsprue , through which metal enters a runner leading to the main cavity </li></ul><ul><li>At the top of downsprue, a pouring cup is often used to minimize splash and turbulence as the metal flows into downsprue </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 20. Riser <ul><li>Reservoir in the mold which is a source of liquid metal to compensate for shrinkage of the part during solidification </li></ul><ul><li>The riser must be designed to freeze after the main casting in order to satisfy its function </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 21. Heating the Metal <ul><li>Heating furnaces are used to heat the metal to molten temperature sufficient for casting </li></ul><ul><li>The heat required is the sum of: </li></ul><ul><ul><li>Heat to raise temperature to melting point </li></ul></ul><ul><ul><li>Heat of fusion to convert from solid to liquid </li></ul></ul><ul><ul><li>Heat to raise molten metal to desired temperature for pouring </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 22. Pouring the Molten Metal <ul><li>For this step to be successful, metal must flow into all regions of the mold, most importantly the main cavity, before solidifying </li></ul><ul><li>Factors that determine success </li></ul><ul><ul><li>Pouring temperature </li></ul></ul><ul><ul><li>Pouring rate </li></ul></ul><ul><ul><li>Turbulence </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 23. Solidification of Metals <ul><li>Transformation of molten metal back into solid state </li></ul><ul><li>Solidification differs depending on whether the metal is </li></ul><ul><ul><li>A pure element or </li></ul></ul><ul><ul><li>An alloy </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 24. Cooling Curve for a Pure Metal <ul><li>A pure metal solidifies at a constant temperature equal to its freezing point (same as melting point) </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 25. Solidification of Pure Metals <ul><li>Due to chilling action of mold wall, a thin skin of solid metal is formed at the interface immediately after pouring </li></ul><ul><li>Skin thickness increases to form a shell around the molten metal as solidification progresses </li></ul><ul><li>Rate of freezing depends on heat transfer into mold, as well as thermal properties of the metal </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 26. <ul><li>Characteristic grain structure in a casting of a pure metal, showing randomly oriented grains of small size near the mold wall, and large columnar grains oriented toward the center of the casting </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e Solidification of Pure Metals
- 27. Solidification of Alloys <ul><li>Most alloys freeze over a temperature range </li></ul><ul><li>Phase diagram for a copper‑nickel alloy system and cooling curve for a 50%Ni‑50%Cu composition </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 28. <ul><li>Characteristic grain structure in an alloy casting, showing segregation of alloying components in center of casting </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e Solidification of Alloys
- 29. Solidification Time <ul><li>Total solidification time T TS = time required for casting to solidify after pouring </li></ul><ul><li>T TS depends on size and shape of casting by relationship known as Chvorinov's Rule </li></ul><ul><li>where T TS = total solidification time; V = volume of the casting; A = surface area of casting; n = exponent with typical value = 2; and C m is mold constant. </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 30. Mold Constant in Chvorinov's Rule <ul><li>Mold constant C m depends on: </li></ul><ul><ul><li>Mold material </li></ul></ul><ul><ul><li>Thermal properties of casting metal </li></ul></ul><ul><ul><li>Pouring temperature relative to melting point </li></ul></ul><ul><li>Value of C m for a given casting operation can be based on experimental data from previous operations carried out using same mold material, metal, and pouring temperature, even though the shape of the part may be quite different </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 31. What Chvorinov's Rule Tells Us <ul><li>Casting with a higher volume‑to‑surface area ratio cools and solidifies more slowly than one with a lower ratio </li></ul><ul><ul><li>To feed molten metal to the main cavity, T TS for riser must be greater than T TS for main casting </li></ul></ul><ul><li>Since mold constants of riser and casting will be equal, design the riser to have a larger volume‑to‑area ratio so that the main casting solidifies first </li></ul><ul><ul><li>This minimizes the effects of shrinkage </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 32. Shrinkage during Solidification and Cooling <ul><li>(0) starting level of molten metal immediately after pouring; (1) reduction in level caused by liquid contraction during cooling </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 33. Shrinkage during Solidification and Cooling <ul><li>(2) reduction in height and formation of shrinkage cavity caused by solidification; (3) further reduction in volume due to thermal contraction during cooling of solid metal </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 34. Solidification Shrinkage <ul><li>Occurs in nearly all metals because the solid phase has a higher density than the liquid phase </li></ul><ul><li>Thus, solidification causes a reduction in volume per unit weight of metal </li></ul><ul><li>Exception: cast iron with high C content </li></ul><ul><ul><li>Graphitization during final stages of freezing causes expansion that counteracts volumetric decrease associated with phase change </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 35. Shrinkage Allowance <ul><li>Patternmakers correct for solidification shrinkage and thermal contraction by making the mold cavity oversized </li></ul><ul><li>Amount by which mold is made larger relative to final casting size is called pattern shrinkage allowance </li></ul><ul><li>Casting dimensions are expressed linearly, so allowances are applied accordingly </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 36. Directional Solidification <ul><li>To minimize effects of shrinkage, it is desirable for regions of the casting most distant from the liquid metal supply to freeze first and for solidification to progress from these regions toward the riser(s) </li></ul><ul><ul><li>Thus, molten metal is continually available from risers to prevent shrinkage voids </li></ul></ul><ul><ul><li>The term directional solidification describes this aspect of freezing and methods by which it is controlled </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 37. Achieving Directional Solidification <ul><li>Directional solidification is achieved using Chvorinov's Rule to design the casting, its orientation in the mold, and the riser system that feeds it </li></ul><ul><ul><li>Locate sections of the casting with lower V / A ratios away from riser, so freezing occurs first in these regions, and the liquid metal supply for the rest of the casting remains open </li></ul></ul><ul><ul><li>Chills ‑ internal or external heat sinks that cause rapid freezing in certain regions of the casting </li></ul></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 38. External Chills <ul><li>(a) External chill to encourage rapid freezing of the molten metal in a thin section of the casting; and (b) the likely result if the external chill were not used </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e
- 39. Riser Design <ul><li>Riser is waste metal that is separated from the casting and remelted to make more castings </li></ul><ul><li>To minimize waste in the unit operation, it is desirable for the volume of metal in the riser to be a minimum </li></ul><ul><li>Since the shape of the riser is normally designed to maximize the V / A ratio, this allows riser volume to be reduced to the minimum possible value </li></ul>©2010 John Wiley & Sons, Inc. M P Groover, Fundamentals of Modern Manufacturing 4/e

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment